CONDIJCTIN& POWEE OF ALLOTS. 
169 
Table VI. (continued.) 
Bismuth-Silver Series. 
Alloy. 
Volume per cent. 
Mean of 
Calculated con- 
ducting power 
from the volume. 
Conducting power. 
Temperature. 
Bi 
^200 
Ag 
99-76 
1*12 
21*3 
1*43 
^'oO 
Ag 
99-04 
1*11 
21*4 
2*14 
i Bi24 
H 
98*01 
1*14 
21*4 
3*16 
Lii2 
Ag 
96*10 
1*32 
19*9 
5*05 
I 
Ag 
92-49 
1*65 
21*6 
8*61 
I 
Ag 
89*15 
1*78 
20*3 
11*92 
Big 
Ag 
80*42 
2*45 
20*1 
20*54 
1 Bi 
Ag 
67*23 
3*30 
21*4 
33*56 
Bi 
Ag2 
50*64 
4*66 
22*4 
49*95 
Bi 
Ag4 
33-91 
8-08 
20*3 
66*49 
Bi and Ag* 
2*33 
47*87 
22*9 
97-70 
* The amount of silver was determined. 
Gold-Copper Series. 
Au and Cu 
Au 
97-72 
46*66 
19-1 
73*34 
Au and Cu 
95-67 
33*01 
19-4 
73*75 
Au and Cu 
91*54 
22*45 
17-9 
74*58 
Au and Cu 
83*83 
1 5*35 
20-3 
76*16 
Au and Cu 
73*15 
12*66 
19-6 
78*32 
Au and Cu 
53*20 
11*45 
17-8 
82*37 
Au and Cu 
38*05 
12*49 
20*1 
85*44 
Au and Cu 
31*07 
14*00 
17*1 
86-91 
Au and Cu 
19-36 
19*86 
16*9 
89-23 
Au and Cu 
11*43 
28*74 
19-5 
90*84 
Au and Cu 
9-06 
33*16 
17-0 
91*32 
Au and Cu 
3*53 
53-18 
18*0 
92*44 
Au and Cu 
1*64 
65*36 
18*1 
92*82 
All hard drawn ; the amount of gold was determined. 
Gold-Silver Series. 
1 
Au84 Ag 
Au 
98*81 
59-09 
25*1 
73*25 
AU56 Ag 
98*23 
53*24 
25*7 
73*41 
Aujfi Ag 
97-27 
48*86 
25*9 
73*67 
Aui6 Ag 
94*07 
38*12 
26*4 
74*54 
Aug Ag 
88-80 
28*58 
26*6 
75*96 
Aug Ag 
85*61 
24*99 
21*5 
76*83 
AU4 Ag 
79-86 
20*91 
21*0 
78*38 
Aug Ag 
66*47 
16*20 
20*2 
82*01 
Au Ag 
49*78 
14*59 
22-2 
86*52 
Au Ag 2 
33*14 
16*30 
19-9 
91*03 
Au Agj 
19-86 
20*94 
21*2 
94*62 
Au Agg 
14*18 
25*29 
19-9 
96*16 
Au Agg 
11*02 
29-87 
19*5 
97-02 
Au Agjg 
5*84 
41*19 
20*5 
98*42 
Au Agjg 
2*68 
56*54 
23*8 
99-27 
Au Agjg 
1*74 
60*63 
21*9 
99-58 
Au Ag84 
1*17 
73*85 
22*1 
99-68 
All hard drawn, not analysed. 
2 A 
MDCCCLX. 
